#------------------------------------------------------------------------------
#$Date: 2021-04-30 11:19:27 +0300 (Fri, 30 Apr 2021) $
#$Revision: 264720 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/23/1562306.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562306
loop_
_publ_author_name
'Li, Na'
'Mu, Bao'
'Cao, Xinyu'
'Huang, Rudan'
_publ_section_title
;
 The structures and properties of the new two-dimensional
 inorganic--organic hybrid materials based on the molybdate chains
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              180
_journal_page_last               186
_journal_paper_doi               10.1016/j.jssc.2014.06.001
_journal_volume                  217
_journal_year                    2014
_chemical_formula_sum            'C16 H20 Co Mo6 N6 O22'
_chemical_formula_weight         1282.95
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                105.944(2)
_cell_angle_beta                 91.9350(13)
_cell_angle_gamma                98.7693(12)
_cell_formula_units_Z            1
_cell_length_a                   7.5923(12)
_cell_length_b                   10.0495(13)
_cell_length_c                   10.2603(12)
_cell_measurement_reflns_used    835
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.1500
_cell_measurement_theta_min      2.7240
_cell_volume                     741.57(17)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0807
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            6281
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         2.72
_exptl_absorpt_coefficient_mu    3.107
_exptl_absorpt_correction_T_max  0.8355
_exptl_absorpt_correction_T_min  0.4364
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    2.873
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             613
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.06
_refine_diff_density_max         3.720
_refine_diff_density_min         -3.211
_refine_diff_density_rms         0.595
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     235
_refine_ls_number_reflns         6281
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.057
_refine_ls_R_factor_all          0.1378
_refine_ls_R_factor_gt           0.1006
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1980P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2692
_refine_ls_wR_factor_ref         0.2959
_reflns_number_gt                4029
_reflns_number_total             6281
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2014-217-180.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1562306
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.20065(14) 0.30870(11) 0.36130(10) 0.0125(3) Uani 1 1 d . . .
Mo2 Mo 0.50044(14) 0.59082(11) 0.37842(10) 0.0106(3) Uani 1 1 d . . .
Mo3 Mo 0.00091(14) 0.57762(11) 0.36344(10) 0.0124(3) Uani 1 1 d . . .
Co1 Co 0.5000 0.5000 0.0000 0.0152(6) Uani 1 2 d S . .
N1 N 0.3911(15) 0.7435(11) -0.0998(12) 0.022(3) Uani 1 1 d . . .
H1 H 0.4250 0.7064 -0.1788 0.027 Uiso 1 1 calc R . .
N2 N 0.4090(16) 0.6947(12) 0.0095(11) 0.022(3) Uani 1 1 d . . .
N3 N 0.1877(16) 1.0633(11) -0.3539(11) 0.022(3) Uani 1 1 d . . .
H3 H 0.1571 1.1040 -0.4126 0.026 Uiso 1 1 calc R . .
O1 O 0.2475(11) 0.5372(9) 0.3829(9) 0.0162(19) Uani 1 1 d . . .
O2 O 0.4576(12) 0.3757(8) 0.4046(8) 0.0121(18) Uani 1 1 d . . .
O3 O -0.0176(12) 0.3741(8) 0.4083(8) 0.0121(18) Uani 1 1 d . . .
O4 O 0.1892(13) 0.2661(9) 0.1876(9) 0.023(2) Uani 1 1 d . . .
O5 O 0.2417(12) 0.4086(10) 0.5850(8) 0.018(2) Uani 1 1 d . . .
O6 O 0.1733(13) 0.1501(10) 0.3968(9) 0.025(2) Uani 1 1 d . . .
O7 O 0.5127(12) 0.5285(9) 0.2073(8) 0.019(2) Uani 1 1 d . . .
O8 O 0.4979(12) 0.7653(9) 0.4065(9) 0.018(2) Uani 1 1 d . . .
O9 O -0.0487(13) 0.4987(11) 0.1953(9) 0.028(2) Uani 1 1 d . . .
O10 O 0.0770(12) 0.7482(10) 0.3753(10) 0.025(2) Uani 1 1 d . . .
O11 O 0.2367(13) 0.4044(10) -0.0090(9) 0.025(2) Uani 1 1 d . . .
H11B H 0.1634 0.4488 -0.0365 0.030 Uiso 1 1 d R . .
H11C H 0.2072 0.3884 0.0651 0.030 Uiso 1 1 d R . .
C1 C 0.3141(19) 0.8561(13) -0.0680(14) 0.021(3) Uani 1 1 d . . .
C2 C 0.2843(19) 0.8856(14) 0.0651(13) 0.022(3) Uani 1 1 d . . .
H2 H 0.2329 0.9596 0.1156 0.026 Uiso 1 1 calc R . .
C3 C 0.3458(19) 0.7836(14) 0.1099(14) 0.022(3) Uani 1 1 d . . .
H3A H 0.3435 0.7776 0.1987 0.026 Uiso 1 1 calc R . .
C4 C 0.282(2) 0.9583(14) -0.3921(14) 0.026(3) Uani 1 1 d . . .
H4 H 0.3166 0.9318 -0.4803 0.031 Uiso 1 1 calc R . .
C5 C 0.3252(19) 0.8912(14) -0.3011(13) 0.023(3) Uani 1 1 d . . .
H5 H 0.3907 0.8185 -0.3275 0.027 Uiso 1 1 calc R . .
C6 C 0.2738(19) 0.9289(14) -0.1679(13) 0.021(3) Uani 1 1 d . . .
C7 C 0.182(2) 1.0426(15) -0.1351(14) 0.025(3) Uani 1 1 d . . .
H7 H 0.1489 1.0751 -0.0470 0.030 Uiso 1 1 calc R . .
C8 C 0.141(2) 1.1055(15) -0.2285(15) 0.029(3) Uani 1 1 d . . .
H8 H 0.0787 1.1803 -0.2046 0.035 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Mo1 O6 104.4(4) . .
O4 Mo1 O3 104.5(4) . .
O6 Mo1 O3 103.1(4) . .
O4 Mo1 O2 100.5(4) . .
O6 Mo1 O2 102.3(4) . .
O3 Mo1 O2 138.2(4) . .
O4 Mo1 O1 92.8(4) . .
O6 Mo1 O1 162.7(4) . .
O3 Mo1 O1 73.0(3) . .
O2 Mo1 O1 72.9(3) . .
O4 Mo1 O5 167.9(4) . .
O6 Mo1 O5 87.1(4) . .
O3 Mo1 O5 75.7(3) . .
O2 Mo1 O5 73.1(3) . .
O1 Mo1 O5 75.7(3) . .
O8 Mo2 O7 104.8(4) . .
O8 Mo2 O1 96.1(4) . .
O7 Mo2 O1 98.1(4) . .
O8 Mo2 O5 101.0(4) . 2_666
O7 Mo2 O5 91.9(4) . 2_666
O1 Mo2 O5 157.3(4) . 2_666
O8 Mo2 O2 89.4(4) . 2_666
O7 Mo2 O2 161.9(4) . 2_666
O1 Mo2 O2 91.3(3) . 2_666
O5 Mo2 O2 74.1(3) 2_666 2_666
O8 Mo2 O2 161.0(4) . .
O7 Mo2 O2 92.5(4) . .
O1 Mo2 O2 73.3(3) . .
O5 Mo2 O2 86.0(3) 2_666 .
O2 Mo2 O2 75.5(3) 2_666 .
O9 Mo3 O10 105.1(5) . .
O9 Mo3 O5 98.1(4) . 2_566
O10 Mo3 O5 99.6(4) . 2_566
O9 Mo3 O1 99.6(4) . .
O10 Mo3 O1 92.3(4) . .
O5 Mo3 O1 155.3(4) 2_566 .
O9 Mo3 O3 91.9(4) . .
O10 Mo3 O3 158.6(4) . .
O5 Mo3 O3 90.5(4) 2_566 .
O1 Mo3 O3 71.8(3) . .
O9 Mo3 O3 163.5(4) . 2_566
O10 Mo3 O3 90.8(4) . 2_566
O5 Mo3 O3 74.3(3) 2_566 2_566
O1 Mo3 O3 84.1(3) . 2_566
O3 Mo3 O3 73.8(3) . 2_566
O7 Co1 O7 180.00(6) 2_665 .
O7 Co1 O11 88.0(3) 2_665 2_665
O7 Co1 O11 92.0(3) . 2_665
O7 Co1 O11 92.0(3) 2_665 .
O7 Co1 O11 88.0(3) . .
O11 Co1 O11 180.000(1) 2_665 .
O7 Co1 N2 84.8(4) 2_665 .
O7 Co1 N2 95.2(4) . .
O11 Co1 N2 90.9(4) 2_665 .
O11 Co1 N2 89.1(4) . .
O7 Co1 N2 95.2(4) 2_665 2_665
O7 Co1 N2 84.8(4) . 2_665
O11 Co1 N2 89.1(4) 2_665 2_665
O11 Co1 N2 90.9(4) . 2_665
N2 Co1 N2 180.0(6) . 2_665
C1 N1 N2 110.3(11) . .
C1 N1 H1 124.9 . .
N2 N1 H1 124.9 . .
C3 N2 N1 105.4(11) . .
C3 N2 Co1 131.0(9) . .
N1 N2 Co1 123.4(8) . .
C8 N3 C4 121.6(12) . .
C8 N3 H3 119.2 . .
C4 N3 H3 119.2 . .
Mo2 O1 Mo3 149.4(5) . .
Mo2 O1 Mo1 106.3(4) . .
Mo3 O1 Mo1 102.8(4) . .
Mo1 O2 Mo2 105.1(4) . 2_666
Mo1 O2 Mo2 104.5(4) . .
Mo2 O2 Mo2 104.5(3) 2_666 .
Mo1 O3 Mo3 106.3(4) . .
Mo1 O3 Mo3 103.3(4) . 2_566
Mo3 O3 Mo3 106.2(3) . 2_566
Mo3 O5 Mo2 154.2(4) 2_566 2_666
Mo3 O5 Mo1 102.8(4) 2_566 .
Mo2 O5 Mo1 102.0(4) 2_666 .
Mo2 O7 Co1 164.8(6) . .
Co1 O11 H11B 112.8 . .
Co1 O11 H11C 113.4 . .
H11B O11 H11C 110.5 . .
N1 C1 C2 108.3(12) . .
N1 C1 C6 122.1(13) . .
C2 C1 C6 129.6(12) . .
C1 C2 C3 105.4(12) . .
C1 C2 H2 127.3 . .
C3 C2 H2 127.3 . .
N2 C3 C2 110.6(12) . .
N2 C3 H3A 124.7 . .
C2 C3 H3A 124.7 . .
N3 C4 C5 119.3(13) . .
N3 C4 H4 120.4 . .
C5 C4 H4 120.4 . .
C4 C5 C6 121.4(13) . .
C4 C5 H5 119.3 . .
C6 C5 H5 119.3 . .
C7 C6 C5 115.6(12) . .
C7 C6 C1 121.5(13) . .
C5 C6 C1 122.9(13) . .
C8 C7 C6 121.0(14) . .
C8 C7 H7 119.5 . .
C6 C7 H7 119.5 . .
N3 C8 C7 121.1(14) . .
N3 C8 H8 119.4 . .
C7 C8 H8 119.4 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O4 1.711(9) .
Mo1 O6 1.714(9) .
Mo1 O3 1.903(9) .
Mo1 O2 1.958(9) .
Mo1 O1 2.216(8) .
Mo1 O5 2.228(8) .
Mo2 O8 1.701(9) .
Mo2 O7 1.706(8) .
Mo2 O1 1.920(9) .
Mo2 O5 1.980(9) 2_666
Mo2 O2 2.163(8) 2_666
Mo2 O2 2.228(8) .
Mo3 O9 1.691(9) .
Mo3 O10 1.693(9) .
Mo3 O5 1.948(9) 2_566
Mo3 O1 1.990(8) .
Mo3 O3 2.202(8) .
Mo3 O3 2.252(8) 2_566
Co1 O7 2.063(8) 2_665
Co1 O7 2.063(8) .
Co1 O11 2.069(9) 2_665
Co1 O11 2.069(9) .
Co1 N2 2.152(11) .
Co1 N2 2.152(11) 2_665
N1 C1 1.319(17) .
N1 N2 1.352(15) .
N1 H1 0.8600 .
N2 C3 1.322(17) .
N3 C8 1.318(18) .
N3 C4 1.341(18) .
N3 H3 0.8600 .
O2 Mo2 2.163(8) 2_666
O3 Mo3 2.252(8) 2_566
O5 Mo3 1.948(9) 2_566
O5 Mo2 1.980(9) 2_666
O11 H11B 0.8500 .
O11 H11C 0.8500 .
C1 C2 1.350(19) .
C1 C6 1.462(17) .
C2 C3 1.367(18) .
C2 H2 0.9300 .
C3 H3A 0.9300 .
C4 C5 1.352(18) .
C4 H4 0.9300 .
C5 C6 1.400(18) .
C5 H5 0.9300 .
C6 C7 1.397(19) .
C7 C8 1.337(19) .
C7 H7 0.9300 .
C8 H8 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
C1 N1 N2 C3 -1.9(15) . . . .
C1 N1 N2 Co1 172.9(9) . . . .
O7 Co1 N2 C3 166.9(13) 2_665 . . .
O7 Co1 N2 C3 -13.1(13) . . . .
O11 Co1 N2 C3 -105.2(13) 2_665 . . .
O11 Co1 N2 C3 74.8(13) . . . .
N2 Co1 N2 C3 -40(100) 2_665 . . .
O7 Co1 N2 N1 -6.5(10) 2_665 . . .
O7 Co1 N2 N1 173.5(10) . . . .
O11 Co1 N2 N1 81.4(10) 2_665 . . .
O11 Co1 N2 N1 -98.6(10) . . . .
N2 Co1 N2 N1 146(100) 2_665 . . .
O8 Mo2 O1 Mo3 22.7(10) . . . .
O7 Mo2 O1 Mo3 -83.2(10) . . . .
O5 Mo2 O1 Mo3 161.4(7) 2_666 . . .
O2 Mo2 O1 Mo3 112.2(9) 2_666 . . .
O2 Mo2 O1 Mo3 -173.4(10) . . . .
O8 Mo2 O1 Mo1 -176.6(4) . . . .
O7 Mo2 O1 Mo1 77.5(5) . . . .
O5 Mo2 O1 Mo1 -37.9(11) 2_666 . . .
O2 Mo2 O1 Mo1 -87.1(4) 2_666 . . .
O2 Mo2 O1 Mo1 -12.7(3) . . . .
O9 Mo3 O1 Mo2 89.5(10) . . . .
O10 Mo3 O1 Mo2 -16.2(10) . . . .
O5 Mo3 O1 Mo2 -135.4(9) 2_566 . . .
O3 Mo3 O1 Mo2 178.4(10) . . . .
O3 Mo3 O1 Mo2 -106.8(9) 2_566 . . .
O9 Mo3 O1 Mo1 -71.5(5) . . . .
O10 Mo3 O1 Mo1 -177.3(4) . . . .
O5 Mo3 O1 Mo1 63.6(9) 2_566 . . .
O3 Mo3 O1 Mo1 17.3(3) . . . .
O3 Mo3 O1 Mo1 92.2(4) 2_566 . . .
O4 Mo1 O1 Mo2 -85.7(5) . . . .
O6 Mo1 O1 Mo2 90.6(14) . . . .
O3 Mo1 O1 Mo2 169.9(5) . . . .
O2 Mo1 O1 Mo2 14.5(4) . . . .
O5 Mo1 O1 Mo2 90.8(4) . . . .
O4 Mo1 O1 Mo3 84.4(5) . . . .
O6 Mo1 O1 Mo3 -99.4(13) . . . .
O3 Mo1 O1 Mo3 -20.0(4) . . . .
O2 Mo1 O1 Mo3 -175.5(4) . . . .
O5 Mo1 O1 Mo3 -99.1(4) . . . .
O4 Mo1 O2 Mo2 -172.9(4) . . . 2_666
O6 Mo1 O2 Mo2 -65.4(4) . . . 2_666
O3 Mo1 O2 Mo2 60.9(6) . . . 2_666
O1 Mo1 O2 Mo2 97.4(4) . . . 2_666
O5 Mo1 O2 Mo2 17.6(3) . . . 2_666
O4 Mo1 O2 Mo2 77.3(4) . . . .
O6 Mo1 O2 Mo2 -175.2(4) . . . .
O3 Mo1 O2 Mo2 -48.9(6) . . . .
O1 Mo1 O2 Mo2 -12.3(3) . . . .
O5 Mo1 O2 Mo2 -92.1(4) . . . .
O8 Mo2 O2 Mo1 72.1(12) . . . .
O7 Mo2 O2 Mo1 -83.5(4) . . . .
O1 Mo2 O2 Mo1 14.2(4) . . . .
O5 Mo2 O2 Mo1 -175.2(4) 2_666 . . .
O2 Mo2 O2 Mo1 110.1(5) 2_666 . . .
O8 Mo2 O2 Mo2 -38.1(13) . . . 2_666
O7 Mo2 O2 Mo2 166.4(4) . . . 2_666
O1 Mo2 O2 Mo2 -95.9(4) . . . 2_666
O5 Mo2 O2 Mo2 74.6(4) 2_666 . . 2_666
O2 Mo2 O2 Mo2 0.0 2_666 . . 2_666
O4 Mo1 O3 Mo3 -70.2(4) . . . .
O6 Mo1 O3 Mo3 -179.1(4) . . . .
O2 Mo1 O3 Mo3 54.8(6) . . . .
O1 Mo1 O3 Mo3 18.3(3) . . . .
O5 Mo1 O3 Mo3 97.4(4) . . . .
O4 Mo1 O3 Mo3 178.3(4) . . . 2_566
O6 Mo1 O3 Mo3 69.3(4) . . . 2_566
O2 Mo1 O3 Mo3 -56.8(6) . . . 2_566
O1 Mo1 O3 Mo3 -93.3(4) . . . 2_566
O5 Mo1 O3 Mo3 -14.2(3) . . . 2_566
O9 Mo3 O3 Mo1 78.9(5) . . . .
O10 Mo3 O3 Mo1 -64.2(11) . . . .
O5 Mo3 O3 Mo1 177.0(4) 2_566 . . .
O1 Mo3 O3 Mo1 -20.6(4) . . . .
O3 Mo3 O3 Mo1 -109.6(5) 2_566 . . .
O9 Mo3 O3 Mo3 -171.5(4) . . . 2_566
O10 Mo3 O3 Mo3 45.4(12) . . . 2_566
O5 Mo3 O3 Mo3 -73.4(4) 2_566 . . 2_566
O1 Mo3 O3 Mo3 89.0(4) . . . 2_566
O3 Mo3 O3 Mo3 0.0 2_566 . . 2_566
O4 Mo1 O5 Mo3 109.0(19) . . . 2_566
O6 Mo1 O5 Mo3 -87.9(5) . . . 2_566
O3 Mo1 O5 Mo3 16.4(4) . . . 2_566
O2 Mo1 O5 Mo3 168.3(5) . . . 2_566
O1 Mo1 O5 Mo3 92.2(4) . . . 2_566
O4 Mo1 O5 Mo2 -78(2) . . . 2_666
O6 Mo1 O5 Mo2 84.7(5) . . . 2_666
O3 Mo1 O5 Mo2 -170.9(5) . . . 2_666
O2 Mo1 O5 Mo2 -19.0(4) . . . 2_666
O1 Mo1 O5 Mo2 -95.2(4) . . . 2_666
O8 Mo2 O7 Co1 -22(2) . . . .
O1 Mo2 O7 Co1 76(2) . . . .
O5 Mo2 O7 Co1 -124(2) 2_666 . . .
O2 Mo2 O7 Co1 -162.7(14) 2_666 . . .
O2 Mo2 O7 Co1 150(2) . . . .
O7 Co1 O7 Mo2 -160(100) 2_665 . . .
O11 Co1 O7 Mo2 95(2) 2_665 . . .
O11 Co1 O7 Mo2 -85(2) . . . .
N2 Co1 O7 Mo2 4(2) . . . .
N2 Co1 O7 Mo2 -176(2) 2_665 . . .
N2 N1 C1 C2 1.7(16) . . . .
N2 N1 C1 C6 -178.4(12) . . . .
N1 C1 C2 C3 -0.7(16) . . . .
C6 C1 C2 C3 179.4(14) . . . .
N1 N2 C3 C2 1.5(16) . . . .
Co1 N2 C3 C2 -172.8(10) . . . .
C1 C2 C3 N2 -0.5(16) . . . .
C8 N3 C4 C5 2(2) . . . .
N3 C4 C5 C6 0(2) . . . .
C4 C5 C6 C7 -2(2) . . . .
C4 C5 C6 C1 178.2(13) . . . .
N1 C1 C6 C7 175.9(13) . . . .
C2 C1 C6 C7 -4(2) . . . .
N1 C1 C6 C5 -5(2) . . . .
C2 C1 C6 C5 175.1(14) . . . .
C5 C6 C7 C8 3(2) . . . .
C1 C6 C7 C8 -177.9(14) . . . .
C4 N3 C8 C7 -2(2) . . . .
C6 C7 C8 N3 -1(2) . . . .
